How to cite this paper: Hu, J.L., Yang, X.S., Shao, L.N., He, X.W. and Men, K.K. (2015) Effect of Alkali Treatment on Heavy Metals Adsorption Capacity of Sewage Sludge. Journal of Geoscience and Environment Protection, 3, 33-39.
Effect of Alkali Treatment on Heavy Metals
Adsorption Capacity of Sewage Sludge
, Xiaosong Yang1
, Linan Shao1
, Xuwen He2
, Kunkuo Men2
1Beijing General Research Institute of Mining & Metallurgy, Beijing, China 2China University of Mining and Technology (Beijing), Beijing, China
Received December 2014
Sewage sludge is the promising raw material for biosorbent preparation. In this work, we eva-luated the heavy metals adsorption characteristics of alkali treated sewage sludge (ATSS) by equi-librium studies. The adsorption isotherms were fitted with Langmuir and Freundlich models. Comparing with untreated sewage sludge, the total adsorption capacity (qm) of ATSS (prepared with 0.125 mol/L NaOH) for Cd, Pb, Ni, increased by 0.51, 0.70 and 0.32 mmol/g, respectively. When the NaOH concentration for ATSS preparation increased from 0.125 mol/L to 0.25 mol/L, the qm of ATSS for Pb decreased from 1.05 mmol/g to 0.84 mmol/g. However, when the NaOH
con-centration increased from 0.25 mol/L to 7.5 mol/L, it showed increasing trend. According to the IR spectra data, the adsorption effect of biosorbent for heavy metals was mainly due to the complex-ation of -N-H groups and -COOH groups.
Sewage Sludge, Alkali Treatment, Heavy Metals, Adsorption
Sewage sludge is an unavoidable by-product of wastewater treatment plants. The costs associated with sludge treatment and disposal can reach 50% of wastewater treatment plants costs . Thus, techniques allowing sludge reduction and resource utilization are increasing studied. Many studies have shown that sewage sludge can ad-sorb substantial quantities of heavy metals in solution -. The bioad-sorbent prepared with sewage sludge can remove heavy metals from wastewater by complex mechanisms including surface complexation with negatively charged biopolymers, ion exchange and physical adsorption -. These mechanisms are influenced by bio-sorbent components and operational conditions: pH, temperature, hydraulic residence time , sludge age , feed C/N ratio , dissolved organic matter , etc.
One of the major problems limiting the real application of biosorbent is that its adsorption capacity for heavy metals is relative low. The heavy metal adsorption capacity of biosorbent made from sewage sludge ranges from 0.01 to 0.38 mmol/g   , it is lower than the commercial adsorbent . The relatively low adsorption capacity of biosorbent means that more biosorbent should be used in order to insure the removal efficiency of
heavy metals in wastewater, and it may produce more wasted biosorbent loaded with heavy metals. Therefore, novel preparation method should be developed in order to improve the adsorption capacity of biosorbent.
The alkali treatment was previously studied as the pretreatment method for sewage sludge anaerobic digestion  , it was proved to be an effective way to enhance the efficiency of biological hydrolysis of sewage sludge and increase methane production -. In addition, it was studied as extraction technique to recover useful organic material (protein, carbohydrates, etc) from sewage sludge -. The alkali treatment can de-stroy the cell walls of bacteria in sewage sludge leading to the solubilization of extracellular and intracellular materials into the aqueous phase. Thus, for sewage sludge, the alkali treatment is possible to enhance the heavy metal adsorption capacity by release of its intracellular complexation sites and chemical modification of func-tion groups. However, to our best knowledge, the adsorpfunc-tion capacity of sewage sludge treated with alkali solu-tion has not been studied. Therefore, the purpose of this study was to investigate the heavy metals adsorpsolu-tion capacity of alkali treated sewage sludge by equilibrium experiments. Furthermore, the effect of alkali concentra-tion for treatment on adsorpconcentra-tion capacity was evaluated as well.
2 Materials and Methods
The sewage sludge was obtained from a municipal wastewater treatment plant in Beijing, China. The sewage sludge was collected after mechanical dewater treatment, stored in refrigerator at −18˚C before use. Main cha-racteristics of sewage sludge are listed in Table 1.
2.2.1. Preparation of Alkali Treated Sewage Sludge
The alkali treated sewage sludge was prepared with NaOH solution of various concentration (range from 0.125 - 7.5 mol/L). Sewage sludge of 25.0 g (approximate dry weight 4.48 g) was added into conical flask containing 100 mL NaOH solution. The suspension was agitated on a shaker at 100 r/min at 35˚C for 12 h. Then, to remove soluble part, the mixture was centrifuged at 6000 × g for 20 min. The solid after centrifugation was collected, added into deionized water and repeated the centrifugation process for twice in order to remove the dissolved impurities and residual NaOH. The final pellet left was suspended in deionized water, neutralized with nitric ac-id solution, diluted to 100 ml with deionized water, and stored at 4˚C before use. This suspension was the alkali treated sewage sludge used in this study.
2.2.2. Adsorption Equilibrium Experiment
Heavy metal adsorption onto alkali treated sewage sludge was evaluated with three typical metals in wastewater: Cadmium (Cd2+), nickel (Ni2+), and lead (Pb2+). All stock solution containing heavy metal were prepared by dissolving heavy metal nitrate salts in deionized water. The pH of heavy metals working solution were adjusted to 5.0 using 0.1 mol/L NaOH solution and 0.1 mol/L nitric acid solution in order to prevent precipitation of heavy metals.
Equilibrium sorption experiments were conducted by adding 10 mL biosorbent to 90 ml heavy metal solution. The mixture was agitated on a rotary shaker at 150 rpm at 25˚C for 24 h. Then the mixture was centrifuged at 6000 × g for 20 min, and the supernatant was filtered with cellulose nitrate membrane (0.45 μm pore size). The filtrate was acidified with concentrated nitric acid and stored at 4˚C before analysis. Blanks without biosorbent were run simultaneously as control. All experimental were run in triplicate. The heavy metals concentration were measured with inductively coupled plasma-atomic emission spectrometry (ICP-AES).
Adsorption experimental data were fitted to the models of Langmuir and Freundlich (Equations (1) and (2), respectively).
1 L m e
K q C q
K C =
+ (1) 1
e F e
q =K C (2) where Ce (mmol/L) is the heavy metal ions concentration at equilibrium, qe (mmol/g) is the amount of adsorbed
Table 1. Main characteristics of sewage sludge.
Property/element Sewage Sludge
Dry matter (wt%) 17.9
Carbon (wt%d) 28.1
Hydrogen (wt%d) 4.2
Oxygen (wt%d) 17.9
Nitrogen (wt%d) 3.8
P (wt%d) 1.2
Sulfur (wt%d) 0.8
Calcium (wt%d) 3.5
Magnesium (wt%d) 5.1
drepresents dry weight element composition.
and n are the isotherm constants.
The adsorption capacity (qe) was calculated as Equation (3).
1 1 2
C V C V V q
where Co (mmol∙L−1) is the initial heavy metal concentration of working solution, Ce (mmol∙L−1) is the
equili-brium concentration of heavy metal, V1 (L) is the volume of working solution, V2 (L) is the volume of biosorbent suspension, m (g) is the dry weight of biosorbent contained in biosorbent suspension. The value of m is meas-ured for every kind of biosorbent suspension.
3. Results and Discussion
3.1. Adsorption Isotherms of Alkali Treated Sewage Sludge
Equilibrium sorption studies were performed to explore heavy metal adsorption capacity of the biosorbent. The adsorption isotherms for sewage sludge and alkali treated sewage sludge were shown in Figure 1 and Figure 2, respectively; qe represented the amount of metal ion adsorbed per unit weight of biomass and Ce represented the
metal ion concentration remaining in solution at equilibrium.
The initial pH value was 5.0 for all working solutions in order to prevent precipitation of heavy metals, the pH was not controlled during the equilibrium experiment. The final pH of heavy metal working solution after ad-sorption was in the range of 5.9 - 6.3 (results are not given). According to previous study , at the pH range of 6, Pb2+ accounts for about 98.6% of total lead, Cd2+ and Ni2+ accounts for 100% of total cadmium and total nickel, respectively. Thus, the precipitation of heavy metal ions can be neglected in the adsorption process.
For both alkali treated sewage sludge and sewage sludge, the Langmuir model yielded a little better fit than the Freundlich model (Table 2), and the good agreement with experimental data suggests that monolayer ad-sorption existed for the experiment, which is consistent with adad-sorption process between heavy metals and other biosorbent such as sugar beet pulp , dried activated sludge . In addition, comparing with sewage sludge, the qm value of alkali treated sewage sludge for Cd, Pb, Ni, increased by 0.51, 0.70 and 0.32 mmol/g,
respec-tively. The higher qm value of alkali treated sewage sludge indicates that the maximum heavy metal adsorption
capacity of sewage sludge was significantly enhanced by alkali treatment.
For alkali treated sewage sludge, qm and KL values followed the order: Pb2+ > Cd2+ > Ni2+. This trend indicates
the bonding affinity of alkali treated sewage sludge to heavy metals is in the order of Pb2+ > Cd2+ > Ni2+.
3.2. Effect of Alkali Concentration on Adsorption Capacity of Sewage Sludge
Figure 1. Heavy metals biosorption isotherms for sewage sludge. Date points are the average of triplicate bottles and the error bars represent standard deviation.
Figure 2. Heavy metals biosorption isotherms for alkali treated sewage sludge (prepared with 0.125 mol/L NaOH). Date points are the average of triplicate bottles and the error bars represent standard deviation.
Table 2. Heavy metals adsorption isotherms parameters for sewage sludge prior to and after alkali treatment (prepared with 0.125 mol/L NaOH).
Langmuir model Freundlich model
adsorbent adsorbate qm (mmol∙g−1) KL (L∙mmol−1) R2 n KF (mmol∙L−1/n∙L1/n∙g−1) R2
Cd2+ 0.25 1.17 0.986 3.25 0.35 0.962
Pb2+ 0.35 3.50 0.982 0.44 2.68 0.936
Ni2+ 0.20 0.52 0.991 0.21 2.15 0.984
Alkali treated sludge
Cd2+ 0.76 21.14 0.993 0.80 3.50 0.947
Pb2+ 1.05 35.09 0.970 1.07 4.69 0.929
Ni2+ 0.52 3.18 0.992 0.55 2.04 0.990
Langmuir model as shown in Table 3, which was consistent with previous study. The principal components in sewage sludge are polysaccharides and proteins. Alkali treatment (mainly NaOH) is an effective carbohydrate and protein extraction method. NaOH ionizes charged groups in proteins and polysaccharides . The ionized functional groups of protein and polysaccharides, such as amino group, hydroxyl group, carboxyl group, com-plexes with heavy metals. Thus, comparing with sewage sludge before treatment, the qm value of treated sewage
sludge prepared by 0.125 mol/L NaOH solution increased by 0.7 mmol/g. However, when the NaOH concentra-tion increased from 0.125 mol/L to 0.25 mol/L, the qm of biosorbent decreased from 1.05 mmol/g to 0.84
mmol/g. This trend may be due to that the NaOH solution with higher concentration hydrolyzed and disinte-grated part of protein and polysaccharides in treated sewage sludge . Nevertheless, when the NaOH concen-tration continued to increase from 0.25 mol/L to 7.5 mol/L, the qm values of treated sewage sludge showed
in-creasing trend. This inin-creasing trend indicates that the NaOH solution with higher concentration leads to the hy-drolysis of bacteria cell of sewage sludge . Then, more intracellular complexation sites expose to heavy metals.
3.3. Functional Groups Analysis
The IR spectra obtained from sewage sludge prior to and after alkali treatment (Figure 4) were used to analysis the presence of main adsorption functional groups. For alkali treated sewage sludge prior to lead adsorption, the peak at 1657 cm−1 was attributed to the stretching vibration of C=O and C-N groups. The peak at 1562 cm−1 was due to the N-H bending vibration and C-N stretching vibration. These groups above were the characteristics spectra of protein. The peak at 1416 cm−1 was assigned to the stretching vibration of C=O and deformation vi-bration of OH. The peak at 1014 cm−1 was attributed to the stretching vibration of OH.
Comparing with the IR spectra of alkali treated sewage sludge prior to and after Pb2+ adsorption, the peak shapes were similar, and no new adsorption peak was observed. It indicated that the material structure did not change after Pb2+ adsorption. After Pb2+ adsorption, the peak at 1570 cm−1 was moved for 20 cm−1 toward infra-
Figure 3. Adsorption isotherms of Pb2+ for biosorbent treated with NaOH solution of different concentration.
Table 3. Pb2+ adsorption isotherms parameters for various alkali treated biosorbent.
Langmuir model Freundlich model
adsorbate qm (mmol∙g−1) KL (L∙mmol−1) R2 n K
F (mmol∙L(1−1/n)∙g−1) R2
0.125 mol/L NaOH treated 1.05 35.09 0.970 1.07 4.69 0.929
0.25 mol/L NaOH treated 0.84 22.81 0.986 0.85 4.81 0.927
2.5 mol/L NaOH treated 1.00 33.27 0.983 1.01 5.08 0.917
Figure 4. IR spectra of untreated sewage sludge and alkali treated sewage sludge.
red region, it was due to the complexation of Pb2+ and N-H group. In addition, the peak at 1408 cm−1 was moved for 32 cm−1 toward infrared region, it was due to Pb2+ binding with -COOH group. Thus, the main function groups works in the heavy metal adsorption process was N-H group and COOH group. These IR spectra data were similar to results of various activated samples obtained by Laurent et al.  .
The alkali treatment is an effective biosorbent preparation method to improve the maximum adsorption capacity of sewage sludge. The alkali treated sewage sludge achieved 1.6 - 2 fold higher adsorption capacity than un-treated sewage sludge. The bonding affinity of alkali un-treated sewage sludge to heavy metals was in the order of Pb2+ > Cd2+ > Ni2+. The increase of heavy metal adsorption capacity was due to the complexation effect of more ionized functional groups formed in the alkali treatment. Furthermore, the alkali treatment leads to hydrolysis of bacteria cell of sewage sludge, and make more intracellular complexation sites expose to heavy metals. Further work is being conducted to determine the suitable operational conditions for usage of alkali treated sewage sludge.
This research was supported by National Natural Science Foundation of China project 51404028 and Beijing General Research Institute of Mining & Metallurgy Research Foundation project YJ-2014-17.
 Apples, L., Baeyens, J., Degreve, J. and Dewil, R. (2008) Principles and Potential of the Anaerobic Digestion of Waste-Activated Sludge. Progress in Energy and Combustion Science, 34, 755-781.
 Li, W.H., Yue, Q.Y., Gao, B.Y., Wang, X.J., Qi, Y.F., Zhao, Y.Q. and Li, Y.J. (2011) Preparation of Sludge-Based Activated Carbon Made from Paper Mill Sewage Sludge by Steam Activation for Dye Wastewater Treatment. Desali-nation, 278, 179-185. http://dx.doi.org/10.1016/j.desal.2011.05.020
 Gascó, G., Méndez, A. and Gascó, J.M. (2005) Preparation of Carbon-Based Adsorbents from Sewage Sludge Pyroly-sis to Remove Metals from Water. Desalination, 180, 245-251. http://dx.doi.org/10.1016/j.desal.2005.01.006
 Otero, M., Rozada, F., Morán, A., Calvo, L.F. and García, A.I. (2009) Removal of Heavy Metals from Aqueous Solu-tion by Sewage Sludge Based Sorbents: Competitive Effects. DesalinaSolu-tion, 239, 46-57.
 Veglio, F. and Beolchini, F. (1997) Removal of Metals by Biosorption: A Review. Hydrometallurgy, 44, 301-316.
Nocardia amarae. Chemosphere, 46, 137-142. http://dx.doi.org/10.1016/S0045-6535(00)00598-1
 Laurent, J., Casellas, M. and Dagot, C. (2009) Heavy Metals Uptake by Sonicated Activated Sludge: Relation with Floc Surface Properties. Journal of Hazardous Materials, 162, 652-660.
 Özbelge, T.A., Özbelge, H.A. and Tursun, M. (2005) Effects of Hydraulic Residence Time on Metal Uptake by Acti-vated Sludge. Chemical Engineering and Processing, 44, 23-32. http://dx.doi.org/10.1016/j.cep.2004.04.004
 Arican, B., Gokcay, C.F. and Yetis, U. (2002) Mechanistics of Nickel Sorption by Activated Sludge. Process Bioche-mistry, 37, 1307-1315. http://dx.doi.org/10.1016/S0032-9592(02)00015-8
 Yuncu, B., Sanin, F.D. and Yetis, U. (2006) An Investigation of Heavy Metal Biosorption in Relation to C/N Ratio of Activated Sludge. Journal of Hazardous Materials, 137, 990-997. http://dx.doi.org/10.1016/j.jhazmat.2006.03.020  Wang, J., Huang, C.P., Allen, H.E., Poesponegoro, I., Poesponegoro, H. and Takiyama, L.R. (1999) Effects of
Dis-solved Organic Matter and pH on Heavy Metal Uptake by Sludge Particulates Exemplified by Copper(II) and Nick-el(II): Three-Variable Model. Water Environment Research, 71, 139-147.
 Laurent, J., Casellas, M., Carrere, H. and Dagot, C. (2011) Effect of Thermal Hydrolysis on Activated Sludge Solubi-lization, Surface Properties and Heavy Metals Biosorption. Chemical Engineering Journal, 166, 842-849.
 Vaughan, T., Seo, C.W. and Marshall, W.E. (2001) Removal of Selected Metal Ions from Aqueous Solution Using Treated Corncobs. Bioresource Technology, 78, 133-139. http://dx.doi.org/10.1016/S0960-8524(01)00007-4
 Li, H., Jin, Y.Y., Mahar, R.B., Wang, Z.Y. and Nie, Y.F. (2008) Effects and Model of Alkaline Waste Activated Sludge Treatment. Bioresource Technology, 99, 5140-5144. http://dx.doi.org/10.1016/j.biortech.2007.09.019
 Dogan, I. and Dilek Sanin, F. (2009) Alkaline Solubilization and Microwave Irradiation as a Combined Sludge Disin-tegration and Minimization Method. Water Research, 43, 2139-2148. http://dx.doi.org/10.1016/j.watres.2009.02.023  Wilson, C.A. and Novak, J.T. (2009) Hydrolysis of Macromolecular Components of Primary and Secondary
Waste-water Sludge by Thermal Hydrolytic Pretreatment. Water Research, 43, 4489-4498. http://dx.doi.org/10.1016/j.watres.2009.07.022
 Lin, J.G., Ma, Y.S. and Huang, C.C. (1998) Alkaline Hydrolysis of the Sludge Generated from a High-Strength, Ni-trogenous-Wastewater Biological-Treatment Process. Bioresource Technology, 65, 35-42.
 Garcia Becerra, F.Y., Acosta, E.J. and Grant Allen, D. (2010) Alkaline Extraction of Wastewater Activated Sludge Biosolids. Bioresource Technology, 101, 6972-6980. http://dx.doi.org/10.1016/j.biortech.2010.04.021
 Liu, H. and Fang, H.H.P. (2002) Extraction of Extracellular Polymeric Substances(EPS) of Sludge. Journal of Bio-technology, 95, 249-256. http://dx.doi.org/10.1016/S0168-1656(02)00025-1
 Sheeng, G. and Yu, Z. (2005) Extraction of Extracellular Polymeric Substances from the Photosynthetic Bacterium
Rhodopseudomonas acidophila. Applied Microbiology and Biotechnology, 67, 125-130. http://dx.doi.org/10.1007/s00253-004-1704-5
 Laurent, J., Pieera, M., Caasellas, M. and Dagot, C. (2009) Fate of Cadmium in Activated Sludge after Changing Its Physicochemical Properties by Thermal Treatment. Chemosphere, 77, 771-777.
 Comte, S., Guibaud, G. and Baudu, M. (2008) Biosorption Properties of Extracellular Polymeric Substances (EPS) to-wards Cd, Cu and Pb for Different pH Values. Journal of Hazardous Materials, 151, 185-193.
 Reddad, Z.C., Gerente, C., Aandres, Y. and Cloirec, P.L. (2002) Adsorption of Several Metal Ions onto a Low-Cost Biosorbent: Kinetic and Equilibrium Studies. Environmental Science & Technology, 36, 2067-2073.
 Wang, X.J., Xia, S.Q., Chen, L., Zhao, J.F., Chovelon, J.M. and Nicole, J.R. (2006) Biosorption of Cadmium(II) and Lead(II) Ions from Aqueous Solutions onto Dried Activated Sludge. Journal of Environmental Sciences, 18, 840-844.  McSwain, B.S., Irvine, R.L., Hausner, M. and Wilderer, P.A. (2005) Composition and Distribution of Extracellular
Polymeric Substances in Aerobic Flocs and Granular Sludge. Applied and Environmental Microbiology, 71, 1051-1057. http://dx.doi.org/10.1128/AEM.71.2.1051-1057.2005